K M Peethambaran et al Int. Journal of Engineering Research and Applications ISSN : 2248-9622, Vol. 4, Issue 4( Version 8), April 2014, pp.06-08 RESEARCH ARTICLE
Anti-Wear Properties of Benzoic Acid in Karanja Oil Anand H*, K M Peethambaran** *(M Tech Scholar (AMD), Dept. of Mechanical Engg, Government College of Engineering Kannur, Kerala670563, India) ** (Professor, Dept. of Mechanical Engg. Government College of Engineering Kannur, Kerala-670563, India)
ABSTRACT Increased concerns about environmental impact caused by mineral oil based lubricants, has created a growing worldwide trend of promoting vegetable oil as base oil for lubricants. . This paper deals with the study of antiwear and anti-friction properties of Karanja (Pongamia Pinnatta) oil and its blends containing numerous amounts of benzoic acid at variable temperatures. The experimental results indicate that Karanja oil and its blends containing benzoic acid, exhibits good anti-wear and anti-friction properties. Keywords - coefficient of friction, four-ball tester, Karanja oil, viscosity index, wear scar diameter ASTM D4172B. For the Viscosity test BROOKFIELD DV2T extra viscometer is used with I. INTRODUCTION international standard ASTM D 2983-03 and VI is There has been growing concern for the use calculated by international standard ASTM Standard of mineral oils as lubricants because of the world D2270-04. Low COF and WSD shows better antiwide environmental issues. This has promoted wear property of oils and high VI shows the better research into developing and using vegetable oils as thermal stability of the oils. alternative base oils for environmentally benign lubricants. Vegetable oils in general have excellent properties such as high viscosity index, high II. EXPERIMENTAL DETAILS lubricity, high flash point, low evaporative loss, high The equipment used for the friction and bio-degradability and low toxicity with regard to their viscosity tests are Four Ball tester TR-30L-PNU-IAS use as base oils for lubricants. On the negative side DUCOM material characterization system, Germany they are known to possess low thermal, oxidative and and BROOKFIELD DV2T extra viscometer, USA, hydrolytic stabilities and poor low-temperature respectively. characteristics. The properties of vegetable oils are Friction and viscosity tests were conducted determined by their fatty acid composition. A high for Karanja oil and its blends containing different content of linoleic/ linolenic acid decreases thermalpercentage of benzoic acid in it. The weight oxidative stability, whereas a higher proportion of concentrations selected are 1%, 1.5%, 2%, 2.5% and long chain saturated fatty acids leads to inferior cold 3% respectively. In four ball tester, tests are flow behavior . conducted under the test conditions of 392N load, 75 0 In this article we have investigated the antiC, 1200 RPM and 3600 seconds. For this test, four wear properties of benzoic acid in Karanja oil. spherical balls used are made of chromium alloy steel Karanja oil is non-edible oil extracted from the seeds and as per specifications laid down in (ASTM D of Karanja (Pongamia Pinnatta) tree. Karanja oil is 2783, 2596, IP 239) and with ANSI standard steel no. widely used in rural India for lighting lamps, as fuel E5100, diameter of 12.7 mm, 64 HN (Hardness for cooking and as medicine for skin diseases. The Number), Grade EP (extra polish) etc. Of the four oilâ€™s non-edible nature and wide availability makes it balls, three are fixed in a ball port and the fourth in a suitable candidate as alternative base oil for motor spindle as shown in Fig.1  lubricants. The physico-chemical, viscometric and other technological properties of Karanja oil which have a bearing on its use as lubricant base oil is scarcely reported in literature. Investigation of antiwear properties predominantly includes the determination of coefficient of friction (COF), wear scar diameter (WSD), and viscosity index (VI). For finding the COF and WSD, tests were conducted on Fig.1: Schematic diagram of four ball geometry Four Ball tester TR-30L-PNU-IAS DUCOM material For calculation of viscosity index, the characterization system with international standard kinematic viscosity of oils at 40 0C and 100 0C is www.ijera.com
K M Peethambaran et al Int. Journal of Engineering Research and Applications ISSN : 2248-9622, Vol. 4, Issue 4( Version 8), April 2014, pp.06-08 determined as per ASTM D445 method. The oil is taken in a container and is heated with the help of silicon oil bath as per the experimental set up in BROOKFIELD DV2T extra viscometer and the corresponding viscosities are found out.
III. RESULTS AND DISCUSSION The results of COF/ WSD and viscosity analysis are given below. The wear scar in the balls is obtained with the help of Transmission Electron Microscope (TEM) and the images for each ball in individual tests indicate the wear scar diameter. Fig. 2 shows wear scar diameter obtained for a ball in one of the tests. The Table 1 shows coefficient of friction and wear scar values of different blends of Karanja oil with various concentrations of benzoic acid. Viscosity index is calculated as follows. First find the kinematic viscosity of oil at 40 0C and 100 0C in centipoises and divide the value with corresponding density value to determine dynamic viscosity at that particular temperature. Then find the values of L and H from table ASTM D 2270-04, corresponding Kinematic Viscosity (at 100 °C) in mm2 /s (centistokes) and calculated the viscosity index with the following formula,
Where, U= kinematic viscosity at 40 °C of the oil, whose viscosity index is to be calculated in mm2/s (centistokes). L = kinematic viscosity at 40 °C of an oil of 0 viscosity index having the same kinematic viscosity at 100 °C as the oil whose viscosity index is to be calculated, mm2/s (centistokes), and H= kinematic viscosity at 40 °C of an oil of 100 viscosity index having the same kinematic viscosity at 100 °C as the oil whose viscosity index is to be calculated, mm2/s (centistokes) .
shows the values of dynamic viscosity at 40 0C and 100 0C and also viscosity index of pure Karanja oil and its different blends with benzoic acid, in different weight percentage. Table 1: Coefficient of friction and wear scar values Sl Weight % COF WSD No Benzoic acid 1 0 0.0551 438.48 2
Table 2: Viscosity of oils at different temperature and viscosity index of various blends of Karanja oil with benzoic acid added in different proportion. % Dynamic Dynamic Viscos Concentra Viscosity Viscosity ity tion at 400c at 1000c index 0 41.77 8.01 147 1 43.56 10.75 162 1.5 53.33 10.53 150 2 51.64 10.54 152 2.5 49.13 10.5 134 3 38.19 8.31 131 The Fig.3 given illustrates the comparison of coefficient of friction graph for different blends of benzoic acid in Karanja oil. This is the wear test view obtained in software WINDCOM, used with four ball tester.
Fig. 3: Comparison of COF graph for different blends of benzoic acid in Karanja oil.
Fig. 2: Wear scar view photograph Table 1 given below shows the COF and WSD values obtained and Table 2 given below www.ijera.com
IV. CONCLUSION Anti-wear properties of Karanja oil were studied for both in the absence and the presence of benzoic acid. Karanja oil provides good anti-wear properties. Four ball tester experimentation is found to a better and easy method for identifying the oil 7|P age
K M Peethambaran et al Int. Journal of Engineering Research and Applications ISSN : 2248-9622, Vol. 4, Issue 4( Version 8), April 2014, pp.06-08
tribological properties like coefficient of friction (COF) and wear scar diameter (WSD). Viscosities obtained in Brookfield viscometer is found to be more accurate than in traditional viscometers. The acquired results indicate that benzoic acid is an effective anti-wear additive for Karanja oil. The friction coefficient and wear scar diameter is significantly reduced by the addition of benzoic acid. The viscosity index is enhanced by the addition of benzoic acid to some extent. The best results are obtained for the oil blend with 2% by weight of benzoic acid.
V. ACKNOWLEDGEMENTS The authors would like to thank Prof. D. Mahipal and Post Graduate student Krishnanunni P, Department of Mechanical Engineering, Govt. Engineering College - Thrissur, Kerala, India, for their support given for the conduct of experiments. The four ball test analysis, viscosity measurement and the recording of the wear scar view were performed at the thermal engineering laboratory of this department.
S A Lawal, et al, “Application of vegetable oil based metalworking fluids”, International Journal of Machine Tools & Manufacture 52, 2012, 1-12. Iman Golsukhnath, et al, “Investigation of Physical Properties for Jatropha Oil in Different Temperature as Lubricant Oil”, Life Science Journal, Vol: 10, 2013, 110119. ASTM INTERNATIONAL - D2270-04 “Standard Practice for Calculating Viscosity Index from Kinematic Viscosity at 40 and 100°C”. Amir SadaKhan, et al, “Antiwear properties of Benzoic acid in bitter rapseed oil and sesame oil at high and low temperature,” International Journal of Mechanical & Mechatronics Engineering IJMME-IJENS Vol:12 No:06, 2012, 7-12. Jayadas, N. H., and Nair, K. P., “Coconut Oil as Base Oil for Industrial LubricantsEvaluation and Modification of Thermal, Oxidative and Low Temperature Properties,” Tribology International, 39, 2006, 873-878.